EFFECT OF COMPOSITION AND MnS ADDITION ON MICROSTRUCTURE AND MECHANICAL PROPERTIES OF POWDER FORGED COPPER STEEL PARTS Ali Haerian Ardakani Department of Materials and Metallurgy, Ferdowsi University of Mashhad Mashhad, Iran, [email protected]
Jalil Vahdati Khaki Department of Materials and Metallurgy, Iran University of Science and Technology Narmak, Tehran, Iran, [email protected]
Hossein Amini Mashhadi
Iranian Academic Center for Education, Culture and Research (ACECR) Iran University of Science and Technology (Received: December 11, 2002 – Accepted in Revised Form: December 25, 2003)
Abstract In this work, the effects of carbon content and manganese sulfide addition on the microstructure and mechanical properties of copper steel parts have been studied. Steel powder mixture containing 2%Cu and different graphite contents with and without MnS additions were compacted, sintered and forged to almost full density. Forged samples, with near theoretical densities, were tested for tensile, hardness, impact and fatigue properties. The microstructures of samples were also studied using optical microscope and scanning electron microscope. It was found that increasing the carbon content did not have any significant effect on fatigue properties of samples, but endurance strength was reduced due to addition of MnS. Furthermore, tensile and yield strength increased by increasing carbon content. Additions of manganese sulfide decreased both tensile and yield strengths but significantly improved the impact energy and elongation of the products. Key Words Powder Forging, Copper Steel, Microstructures, Mechanical Properties, MnS Addition
ﭼﻜﻴﺪﻩ ﺩﺭ ﺍﻳﻦ ﺗﺤﻘﻴﻖ ﺗﺎﺛﻴﺮ ﻣﻴﺰﺍﻥ ﻛﺮﺑﻦ ﻭ ﺍﻓﺰﻭﺩﻥ ﺳﻮﻟﻔﻴﺪ ﻣﻨﮕﻨﺰ ﺭﻭﻱ ﺭﻳﺰ ﺳﺎﺧﺘﺎﺭ ﻭ ﺧﻮﺍﺹ ﻣﻜﺎﻧﻴﻜﻲ ﻗﻄﻌﺎﺕ ﭘﻮﺩﺭ ﻣﺲ ﻭ ﻣﻘﺎﺩﻳﺮ ﻣﺘﻔﺎﻭﺗﻲ ﺍﺯ ﭘﻮﺩﺭ ﮔﺮﺍﻓﻴﺖ ﺩﺭ ﺩﻭ%٢ ﭘﻮﺩﺭ ﺁﻫﻦ ﻫﻤﺮﺍﻩ ﺑﺎ.ﻓﻮﻻﺩﻱ ﻣﺲ ﺩﺍﺭ ﻣﻄﺎﻟﻌﻪ ﺷﺪﻩ ﺍﺳﺖ ﺳﭙﺲ ﺗﻒ ﺟﻮﺷﻲ ﮔﺸﺘﻪ ﻭ ﻧﻬﺎﻳﺘﺎ" ﺗﺎ، ﭘﺲ ﺍﺯ ﻣﺨﻠﻮﻁ ﻧﻤﻮﺩﻥ ﻓﺸﺮﺩﻩ ﺷﺪﻩ،ﺣﺎﻟﺖ ﻫﻤﺮﺍﻩ ﺑﺎ ﺍﻓﺰﻭﺩﻥ ﺳﻮﻟﻔﻴﺪ ﻣﻨﮕﻨﺰ ﻧﻤﻮﻧﻪ ﻫﺎﻱ ﺁﻫﻨﮕﺮﻱ ﺷﺪﻩ ﺗﺤﺖ ﺁﺯﻣﺎﻳﺸﻬﺎﻱ ﺧﻮﺍﺹ ﻣﻜﺎﻧﻴﻜﻲ.ﺭﺳﻴﺪﻥ ﺑﻪ ﭼﮕﺎﻟﻲ ﻛﺎﻣﻞ )ﺗﺌﻮﺭﻱ( ﺁﻫﻨﮕﺮﻱ ﺷﺪﻧﺪ ﻫﻤﭽﻨﻴﻦ ﺭﻳﺰ ﺳﺎﺧﺘﺎﺭ ﻧﻤﻮﻧﻪ ﻫﺎ ﺗﻮﺳﻂ ﻣﻴﻜﺮﻭﺳﻜﻮﭖ. ﻗﺮﺍﺭ ﮔﺮﻓﺘﻨﺪ، ﺿﺮﺑﻪ ﻭ ﺳﺨﺘﻲ ﺳﻨﺠﻲ، ﺧﺴﺘﮕﻲ،ﺷﺎﻣﻞ ﻛﺸﺶ ﺑﺎ ﺑﺮﺭﺳﻴﻬﺎﻱ ﺑﻌﻤﻞ.ﻧﻮﺭﻱ ﻭ ﺳﻄﺢ ﻣﻘﺎﻃﻊ ﺷﻜﺴﺖ ﻧﻴﺰ ﺗﻮﺳﻂ ﻣﻴﻜﺮﻭﺳﻜﻮﭖ ﺍﻟﻜﺘﺮﻭﻧﻲ ﻣﻮﺭﺩ ﻣﻄﺎﻟﻌﻪ ﻗﺮﺍﺭ ﮔﺮﻓﺘﻨﺪ ﻭﻟﻲ ﺑﺎ ﺍﻓﺰﻭﺩﻥ ﺳﻮﻟﻔﻴﺪ.ﺁﻣﺪﻩ ﻣﺸﺨﺺ ﮔﺮﺩﻳﺪ ﻛﻪ ﺍﻓﺰﺍﻳﺶ ﻣﻴﺰﺍﻥ ﻛﺮﺑﻦ ﺗﺎﺛﻴﺮ ﭼﻨﺪﺍﻧﻲ ﺭﻭﻱ ﺧﻮﺍﺹ ﺧﺴﺘﮕﻲ ﻧﺪﺍﺭﺩ ﺍﻣﺎ ﺍﻓﺰﺍﻳﺶ ﻣﻴﺰﺍﻥ ﻛﺮﺑﻦ ﺑﺎﻋﺚ ﺍﻓﺰﺍﻳﺶ ﺍﺳﺘﺤﻜﺎﻡ ﺗﺴﻠﻴﻢ ﻭ ﺍﺳﺘﺤﻜﺎﻡ. ﺍﺳﺘﺤﻜﺎﻡ ﺧﺴﺘﮕﻲ ﻛﺎﻫﺶ ﭘﻴﺪﺍ ﻣﻲ ﻛﻨﺪ،ﻣﻨﮕﻨﺰ ﻭﻟﻲ ﺑﻄﻮﺭ، ﻫﻤﭽﻨﻴﻦ ﻋﻠﻴﺮﻏﻢ ﺍﻳﻨﻜﻪ ﺍﻓﺰﻭﺩﻥ ﺳﻮﻟﻔﻴﺪ ﻣﻨﮕﻨﺰ ﺑﺎﻋﺚ ﻛﺎﻫﺶ ﺍﻳﻦ ﺩﻭ ﭘﺎﺭﺍﻣﺘﺮ ﻣﻲ ﮔﺮﺩﺩ.ﻛﺸﺶ ﻣﻲ ﺷﻮﺩ .ﻗﺎﺑﻞ ﺗﻮﺟﻬﻲ ﻣﻨﺠﺮ ﺑﻪ ﺑﻬﺒﻮﺩ ﺍﻧﺮﮊﻱ ﺟﺬﺏ ﺷﺪﻩ ﺩﺭ ﺁﺯﻣﺎﻳﺶ ﺿﺮﺑﻪ ﻭ ﺍﻓﺰﺍﻳﺶ ﺩﺭﺻﺪ ﺍﺯﺩﻳﺎﺩ ﻃﻮﻝ ﻧﻤﻮﻧﻪ ﻫﺎ ﻣﻲﮔﺮﺩﺩ
1. INTRODUCTION Powder forging of iron-based powders has been the subject of intensive study with the aim of replacing conventionally forged parts, especially those used in automobiles. Hot forging of the IJE Transactions B: Applications
sintered pre-form is carried out to reduce the porosity and hence, improve mechanical (especially dynamic) properties of the parts . If the density of final product reaches close to that of the theoretical value (i.e. 0% porosity or pore-free material), mechanical properties of powder Vol. 17, No. 1, April 2004 - 81
TABLE 1. Chemical Analysis of the Atomized Iron Steel Powder.
Type of Powder
Elements Row Rate Density Sec/50gr C (Max) Si (Max) Mn (Max) P (Max) S (Max) Cu (gr/cm3)
H2 Loss Mo -
TABLE 2. Size Distribution of Powder (Mass Fraction).
Particle Size Distribution
Subsieve (Weight%) 63-100 100-160 31
need extensive machining after forging and heat treatment, good mach inability is crucial. Addition of soft materials such as manganese sulfide can greatly enhance mach inability of these materials, but it has the disadvantage of reducing the dynamic properties through formation of stress concentration sites. The potential for reducing dynamic properties, greatly depends on size, size distribution, and location of these inclusions . Therefore, if these parameters can be controlled properly, mach inability may be improved without sacrificing vital mechanical properties.
forged material can be superior to that of the conventionally forged one . Presence of as much as 0.1% free pores reduces the UTS of quenched and tempered high alloy material (i.e. P/F 4650), but if oxygen and sulfur content is controlled (less than 0.005% O2 and less than 0.1% S), UTS of over 1800 MPa with 40% elongation of 2 inch tensile specimen may be achieved . However, presence of impurities, especially non-metallic inclusion, can adversely affect mechanical properties . This paper is a part of a research project related to the replacement of pre-alloyed powder containing various alloying elements such as Ni and Mo to replace Astalloy D with the mixture of elemental powder containing graphite and copper for producing the load-bearing parts. The paper gives an account of study of the effect of various graphite and MnS contents on the fracture behavior and mechanical properties of powder forged copper steel parts. All specimens were produced in a similar procedure for pre-alloyed part to achieve the real result. Amongst various standard powder forged (P/F) materials , P/F-10Cxx and P/F-11Cxx series (i.e. copper steels) have proved to be suitable materials for load-bearing parts such as cam lobes and connecting rods [6-9]. However, for parts that
Type of Powder WPL-200
82 - Vol. 17, No. 1, February 2004
2. EXPERIMENTAL PROCEDURES
Iranian made iron powder was used as a base for production of 120×30×12 mm forged blanks. This is a water atomized and hydrogen-annealed powder with chemical composition as given in Table 1, and size distribution in Table 2. Four different mixtures with compositions given in Table 3 were prepared by mixing the iron powder with 2% copper and different amounts of graphite and MnS. The characteristics of copper powder are shown in Table 4. The average particle IJE Transactions B: Applications
TABLE3. Chemical Composition of Starting Powders.
Cu 2.00 2.00 2.00 2.00
1 2 3 4
Chemical composition (%) C MnS 0.50 0.00 0.50 0.35 0.75 0.00 0.75 0.35
Fe Bal. Bal. Bal. Bal.
TABLE 4. Characteristics of Copper Powder.
Characteristic Sieve Analysis ISO 4497 >63µm
Oxygen ISO 4491/4
0.8 94.1 1.58 0.13
Apparent Density ISO 3923/2
size of MnS was about 5-7 µm. In order to avoid segregation of low-density graphite, copper and MnS were added to iron powder and mixed for 30 minutes before adding graphite. Graphite was used in the form of ultra-fine powder. 0.8% zinc stearate was used as lubricant. Mixed powders were shaped into blocks and subjected to the sintering and forging regimes described below. Specimens were sintered at 1120ºC in a 75% H2-25%N2 atmosphere for almost 40 minutes. The specimens, after heating to the forging temperature, (about 1100 ºC) were transferred quickly (in less than seven seconds) into the 450 ton forging press and forged to near-full density with no lateral flow. Finally, samples were cooled very slowly in a protected atmosphere (N 2 atmosphere). The emerging samples were at temperatures of around 50 ºC. 2.2. Specimen Preparation Each forged block was sectioned, cut, and machined to appropriate size for mechanical and microstructure studies.
IJE Transactions B: Applications
Mechanical Tests Hardness Tests: Five Vickers measurements (HV 30) were taken on each specimen. The average of these measurements was recorded as the hardness value of material. Tensile Tests: tensile tests were carried out on at least two specimens according to ASTM A 370 and the average value recorded as the strength and elongation of the material. Impact Tests: Charpy V-notch tests were carried out at room temperature on two specimens of each material and the average value recorded as the impact energy of the material. Impact tests were carried out on a 300J impact-testing machine. Fatigue Tests: A bench type rotation-bending fatigue testing machine with a shaft speed 12000 rotations per minute and R value-1 used at room temperature according to the test standard ISO 2740-1973 . Specimens that completed 3×106
Vol. 17, No. 1, April 2004 - 83
TABLE 5. Mechanical Properties of Alloys used in This Research.
Micro structural Studies
specimens with and without MnS. Impact Strength The Charpy impact value of 3 joules for notched specimen of samples containing 0.5% carbon is rather low, but can be increased to 4 joules by addition of 0.35% MnS. Hardness Figure 2 shows the change in hardness due to addition of MnS at both carbon levels. This effect is more clearly shown in Figure 3.
Optical Microscopy: Specimens, both after sintering and forging, were sectioned, ground and polished to 0.3-micrometer finish. These specimens were etched and studied with an optical microscope.
cycles without failure were termed run-out specimens.
Elongation % %Change
Yield Strength (MPa) %Change
Scanning Electron Microscopy (SEM): Fractured surfaces of tensile and impact specimens were examined at ×500 and ×1000 magnifications.
3. RESULTS AND DISCUSSION
The chemical analysis of forged powder samples was determined by quantometric analysis. It has been found that there has been average of about 22% carbon loss in the samples (test bars).
Density after Forging Density of the forged materials was measured 7.80±0.02 gr/cm3. Porosity as determined from the randomly chosen specimens was between 0.1 to 0.4%, which is tolerable for most applications.
Results of tests for mechanical properties and variations of these properties with respect to the composition are listed in Table 5. Figure 1 shows changes of strength and elongation with carbon content for
84 - Vol. 17, No. 1, February 2004
Fatigue properties for three of the four alloys are shown in Figure 4. It is found that increasing carbon content from 0.5% to 0.75% (Alloys 1 and 3) does not have significant effect on the endurance strength.
The test bars were subjected to metallographic examinations. The typical unetched microstructure of MnS-free material (Alloy 1) is presented in Figure 5. No porosity is seen at a magnification of ×200 and only a few small inclusions,